Abstract
Extensive work on single molecule magnets has identified a fundamental mode of relaxation arising from the nuclearspin assisted quantum tunnelling of nearly independent and quasiclassical magnetic dipoles. Here we show that nuclearspin assisted quantum tunnelling can also control the dynamics of purely emergent excitations: magnetic monopoles in spin ice. Our low temperature experiments were conducted on canonical spin ice materials with a broad range of nuclear spin values. By measuring the magnetic relaxation, or monopole current, we demonstrate strong evidence that dynamical coupling with the hyperfine fields bring the electronic spins associated with magnetic monopoles to resonance, allowing the monopoles to hop and transport magnetic charge. Our result shows how the coupling of electronic spins with nuclear spins may be used to control the monopole current. It broadens the relevance of the assisted quantum tunnelling mechanism from single molecular spins to emergent excitations in a strongly correlated system.
Introduction
In the canonical dipolar spin ice materials (Dy_{2}Ti_{2}O_{7}, Ho_{2}Ti_{2}O_{7})^{1,2,3,4}, rare earth ions with total angular momentum J = 15/2 (Dy^{3+}) and J = 8 (Ho^{3+}) are densely packed on a cubic pyrochlore lattice of cornerlinked tetrahedra. The ions experience a very strong 〈111〉 crystal field, resulting in two effective spin states (M_{J} = ±J) that define a local Isinglike anisotropy. At the millikelvin temperatures discussed here (0.08 K < T < 0.2 K), a lattice array of such large and closely spaced spins would normally be ordered by the dipole–dipole interaction^{5}, but the pyrochlore geometry of spin ice frustrates the dipole interaction and suppresses longrange order. Instead, the system is controlled by an icerule, that maps to the Pauling model of water ice^{1,2,3,4}. In the effective ground state, the spins describe a flux with closedloop topology and critical correlations, that may be described by a local gauge symmetry rather than by a traditional broken symmetry^{6}. This strongly correlated spin ice state is stabilised by a remarkable selfscreening of the dipole interaction^{7,8}. Excitations out of the spin ice state fractionalise to form effective magnetic monopoles^{6,9}, but the excited states are no longer selfscreened and this manifests as an effective Coulomb interaction between monopoles. The static properties of spin ice are accurately described by the monopole model^{10}. The dynamic properties can also be described by assuming an effective monopole mobility^{11,12,13}, but there have been few studies of the microscopic origin of the monopole motion^{14}.
The field and energy scales involved in monopole motion are illustrated in Fig. 1a–e. When a monopole hops to a neighbouring site a spin is flipped (Fig. 1a). For an isolated monopole (far from any others) this spin flip takes place at nominally zero energy cost (Fig. 1b) because contributions from nearneighbour antiferromagnetic superexchange and ferromagnetic dipole–dipole coupling individually cancel. The cancellation of the field contribution relies on the dipolar selfscreening^{8} that maps the longrange interacting system^{7} to the degenerate Pauling manifold of the near neighbour spin ice model^{2}. This surprising cancellation is a key result of the manybody physics of spin ice. In practice, a monopole hop may also involve a finite energy change arising from longitudinal fields at the spin site: the main source of fields is nearby monopoles^{6} (Fig. 1b), while further contributions arise from corrections to the mapping, which give a finite energy spread to the Pauling manifold^{15} (here of order ~0.1 K^{16}). The mechanism of the hop is believed to be quantum tunnelling and several key signatures of this have been observed in the high temperature regime between 2 and 10 K^{12,13,14,17,18}.
At lower temperatures (T < 0.6 K), spin ice starts to freeze^{18}. This is due in part to the rarefaction of the monopole gas whose density n(T) varies as ~e^{−μ/T} where the chemical potential μ = 4.35 and 5.7 K for Dy_{2}Ti_{2}O_{7} and Ho_{2}Ti_{2}O_{7}, respectively^{6}, and also in part to geometrical constraints that create noncontractable, monopole–antimonopole pairs that cannot easily annihilate^{19}. These factors, which are independent of the monopole hopping mechanism, suggest that the relaxation rate ν(T) ∝ n(T) will fall to exponentially small values at low temperature (T < 0.35 K).
Previous thermal quenching experiments have demonstrated monopole populations well below the nominal freezing temperature that are both long lived and able to mediate magnetic relaxation^{20}. This paradoxical frozen but dynamical character of the system suggests the relevance of resonant magnetic tunnelling, where magnetisation reversal can only occur when the longitudinal field is smaller than the tunnelling matrix element ΔE. The monopolar fields may add a longitudinal component that takes the spin off the resonance condition (Fig. 1c, d) but in addition may add a transverse component that amplifies ΔE: together these lead to a suppression and dispersion of the monopole mobility.
In the following, we will demonstrate experimentally that hyperfine interactions (Fig. 1e) play a significant role in bringing monopoles back to their resonance condition, enabling dynamics at very low temperatures (T < 0.35 K).
Results
Samples
To investigate the effect of nuclear spins on the magnetic relaxation in spin ice, we studied four spin ice samples: Ho_{2}Ti_{2}O_{7}, with I = 7/2 and three Dy_{2}Ti_{2}O_{7} samples spanning a range of nuclear spin composition from I = 0 to I = 5/2. Details of nuclear spins and hyperfine parameters are given in Table 1. Ho^{3+} is a nonKramers ion with intrinsically fast dynamics owing to the possibility of transverse terms in the singleion spin Hamiltonian, while Dy^{3+}, being a Kramers ion, has intrinsically much slower dynamics. However, it should be noted that, at low temperature, bulk relaxation is slower in Ho_{2}Ti_{2}O_{7} than in Dy_{2}Ti_{2}O_{7}, owing to its larger μ and hence much smaller monopole density (see Supplementary Fig. 1).
Thermal protocol
In previous experiments we have accurately manipulated the monopole density in Dy_{2}Ti_{2}O_{7} by rapid magnetothermal cooling (Avalanche Quench Protocol, AQP) the sample through the freezing transition, allowing the controlled creation of a nonequilibrium population of monopoles in the frozen regime^{20}. However, it is more problematic to cool samples containing Ho, due to the large Ho nuclear spin which results in a Schottky heat capacity of 7 J mol^{−1} K^{−1} at 300 mK. Indeed this anomaly has been exploited by the Planck telescope where the bolometers are attached to the cold plate by yttrium–holmium feet thus allowing passive filtering with a several hour time constant that was crucial to the operation of the system^{21}. For Ho_{2}Ti_{2}O_{7} this means difficulty in cooling. Therefore, during some of the runs the sample temperature was recorded via a thermometer directly mounted on the sample face. Figure 2a shows the monitoring of the sample temperature as it approaches equilibrium for Ho_{2}Ti_{2}O_{7} and Dy_{2}Ti_{2}O_{7} during and after the AQP. The inset of Fig. 2a shows that only a few seconds are required to cool the samples from 0.9 to 0.2 K, which is well below the freezing transition. Whereas Dy_{2}Ti_{2}O_{7} continues to cool, reaching 80 mK after only 10 s, Ho_{2}Ti_{2}O_{7} takes nearly 2000 s to reach the same temperature. Hence, the data shown here were taken at 80 mK for Dy_{2}Ti_{2}O_{7} and 200 mK (and 80 mK when possible) for Ho_{2}Ti_{2}O_{7}.
Monopole density
We have phenomenologically estimated how the monopole density depends upon the rate of sample cooling, dT/dt and the spin relaxation time τ(T) = 1/ν(T), which is derived from the peaks in the imaginary component of the ac susceptibility. Differentiation of τ(T) to give dτ/dT and hence dT/dτ, allows definition of an equilibrium cooling rate dT/dτ, that gives the maximum cooling rate that may still maintain equilibrium. Figure 2b compares dT/dt and dT/dτ for both Dy_{2}Ti_{2}O_{7} and Ho_{2}Ti_{2}O_{7}. It can be seen that after the AQP, dT/dt for Ho_{2}Ti_{2}O_{7} crosses the equilibrium curve and goes out of equilibrium at ≈0.9 K, and for Dy_{2}Ti_{2}O_{7} at ≈0.72 K. The upper limit of the monopole density at low temperature can be estimated by equating it to the theoretical value at the crossing temperature: thus we find one monopole on approximately every 10^{3} tetrahedra for both Ho_{2}Ti_{2}O_{7} and Dy_{2}Ti_{2}O_{7}.
Spontaneous relaxation
We studied the effect of wait time t_{w} between the end of the avalanche quench and the application of the field with the aim to determine the effect of nuclear spins on the monopole dynamics. Varying the wait time deep in the frozen regime allowed us to gauge the spontaneous evolution of the zerofield monopole density as a function of time: that is, if monopoles recombine in a time t_{w}, then the observed monopole current will be smaller, the longer the wait time. Two separate experiments were designed to study these effects. In the first experiment (Fig. 3) after waiting we applied a constant field and measured the magnetisation M as a function of time. In the second experiment (Fig. 4) we investigated the effect of wait time on the magnetothermal avalanches^{22,23,24} that occur on ramping the field to high values. Both of these allowed access to the magnetic current density J_{m} = dM/dt. Full details of the experimental conditions are given in Supplementary Note 1 and Supplementary Fig. 2.
The monopole current is controlled by multiple factors. In the simplest model^{9} there are three of these: the monopole density n, the monopole mobility u (related to the spin tunnelling rate) and the bulk susceptibility χ. Thus J_{m} = dM/dt = ν(M_{eq} − M) where M_{eq} = χH is the equilibrium magnetisation and ν ∝ un. In general it is difficult to deconvolve these various factors. In ref. ^{13} it was achieved by independent measurement of n(T) and χ(T) to reveal u(T). In the present timedependent experiments we cannot perform such a direct separation, but by studying Dy_{2}Ti_{2}O_{7} samples with different isotopes, it seems reasonable to assume that the susceptibility and starting density are roughly the same, so the variation in mobility (hop rate) will dominate differences between the samples. Inclusion of Ho_{2}Ti_{2}O_{7} in the comparison gives a further point of reference: the starting monopole densities (see above) and susceptibilities for Ho_{2}Ti_{2}O_{7} are expected to be comparable to those of Dy_{2}Ti_{2}O_{7}, while the tunnel splitting (which controls the intrinsic mobility) is also estimated to be of the same order^{14} in the appropriate range of internal fields (see Fig. 1 and ref. ^{14}, Fig. 5).
Figure 3 summarises results for the relaxation of the magnetisation M(t) for the different samples, as well as the value of M(t = 400 s) and the monopole current J_{m}(t = 0) as a function of wait time, for a constant applied field of 0.08 T. The Dy_{2}Ti_{2}O_{7} samples show a clear progression in wait time effect that correlates strongly with their relative densities of nuclear spin states. Thus the monopoles recombine during the wait period much more effectively the larger the nuclear spin: that is, the larger the nuclear spin the higher the monopole mobility, the faster the recombination, and the fewer the monopoles at the start of the measurement. In Fig. 3e, f, higher mobility means the relaxation curves (M(t = 400 s) and J_{m}(t = 0)) shift both up and to the left, so a crossover in curves is expected—and this is indeed observed at the longer times. Near to equilibrium a second crossover would be expected (i.e., the equilibrium current density is higher for the highest mobility), but this crossover is clearly very far outside our time window. Hence our Dy_{2}Ti_{2}O_{7} samples are always far from equilibrium.
The effects observed for Dy_{2}Ti_{2}O_{7} are yet more dramatic in Ho_{2}Ti_{2}O_{7}, consistent with the Ho^{3+} nonKramers character, large nuclear spin, and large hyperfine coupling. Relaxation at 200 mK covers more than two orders of magnitude but is practically extinguished for long wait times, showing that excess monopoles spontaneously recombine to eliminate themselves from the sample. The plots indicate that the half life for monopole recombination in Ho_{2}Ti_{2}O_{7} would be approximately 150 s (much shorter than the equilibrium relaxation time) and suggests that equilibrium in the monopole density is reached at long times. Using the above estimate for the initial monopole density n(t = 0) ~ 10^{−3}, we recover a nominal equilibrium density of n_{eq} = 10^{−5} (per rare earth atom). Although this estimate is an upper limit it is nevertheless far from the expected equilibrium density, \(n_{{\mathrm{eq}}}{{\mathrm{(T=200}}\,{\mathrm{mK)}}}\sim 10^{  13}\) (calculated by the method of ref. ^{10}, see Supplementary Fig. 1). It continues to evolve with temperature, being lower by a further order of magnitude at T = 80 mK (Fig. 3f). Most likely, the actual equilibrium monopole density is amplified by defects and disorder in the sample.
Magnetothermal avalanches
Figure 4 illustrates the effect of t_{w} on the magnetothermal avalanches. These occur when the injected power (μ_{0}H × J_{m}) overwhelms the extraction of thermal energy from the sample to the heat bath^{23} such that monopoles are excited in great excess as the temperature steeply rises. The faster and more abundant the monopoles, the lower the avalanche field. To obtain the data in Fig. 4, after the AQP and t_{w}, the applied field was swept at a constant rate, 0.02 T s^{−1} up to 0.4 T. If the avalanche field H_{ava}(t_{w}), is defined as the field where the magnetisation crosses 1μ_{B} per rare earth ion, (0.5μ_{B} for the ^{163}Dy sample) then the difference in avalanche field ΔH_{ava} = H_{ava}(t_{w}) − H_{ava}(t_{w} = minimum) allows us to compare the spread of fields for all samples.
Figure 4a, b shows the experimental results for the isotopically enriched Dy_{2}Ti_{2}O_{7} samples at 80 mK, demonstrating a very clear pattern. In general the spread of H_{ava}(t_{w}) becomes larger, the larger the nuclear spin, showing again that the nuclear spins strongly enhance the monopole mobility. Thus, the ^{162}Dy sample (no nuclear spin) shows negligible evolution of the position of the avalanche field. For ^{nat}Dy_{2}Ti_{2}O_{7} (shown in Supplementary Fig. 4) the effect is small, while for the ^{163}Dy sample (maximum nuclear spin) the effect of t_{w} can be clearly seen as a steady progression of H_{ava}(t_{w}) to higher fields for increasing t_{w} due to the smaller initial monopole density at the start of the field ramp. Also shown in the figure are the curves that result from slow conventional zero field cooling (CC) from 900 to 80 mK (at 1 mK s^{−1}) followed by a 1000 s wait period. For the ^{162}Dy and ^{nat}Dy_{2}Ti_{2}O_{7} samples the CC avalanche field is offset to higher fields, well outside the distribution of H_{ava}(t_{w}). For the ^{163}Dy sample the CC curves falls within the distribution but near the long wait time curves. Also, we note for ^{163}Dy, that in a second measurement with better thermal contact, and thus faster cooling during the AQP, the CC curve again falls outside the distribution (shown in Supplementary Fig. 10b). Thus slow cooling is more efficient at approaching equilibrium in Dy_{2}Ti_{2}O_{7} than is the AQP cooling followed by a long t_{w}, especially for the lownuclear moment samples. This is typical behaviour for frustrated or disordered systems because slow cooling allows the system time to explore all available phase space.
Figure 4c shows a much greater effect of t_{w} for Ho_{2}Ti_{2}O_{7} with a larger spread of fields, saturating near 0.32 T for the longest t_{w}. This is again consistent with the conclusion that the larger the nuclear spin moment, the more effective the spontaneous monopole recombination. The measurements were performed primarily at 200 mK, but the same conclusion follows from measurements at 80 mK. Ho_{2}Ti_{2}O_{7} also exhibits some unusual behaviour suggesting that the monopole density and magnetisation do not approach equilibrium in a simple way. First, the magnetisation jumps fall short of the M vs. H equilibrium curve taken at 900 mK, even though thermometers placed on the sample indicate that the sample does indeed heat above 900 mK (see Supplementary Note 2 and Supplementary Fig. 3 for more details). Secondly, in contrast to the behaviour of Dy_{2}Ti_{2}O_{7} discussed above, the CC curve of Ho_{2}Ti_{2}O_{7} falls in the middle of the distribution of H_{ava}(t_{w}) indicating, unusually, that waiting long enough at low temperature is an equally efficient way of approaching equilibrium as slow cooling.
Discussion
The experimental result demonstrated here is that magnetic monopole dynamics in the frozen regime of spin ice are greatly enhanced by the hyperfine coupling of the electronic and nuclear moments. We now argue that this observation finds a natural—albeit surprising—explanation by analogy with the properties of singlemolecule magnets^{25}. These are metal–organic clusters with large composite spins: some of the most studied include the so called Mn_{12} and Fe_{8} systems, both of which can be thought of as an ensemble of identical, weakly interacting nanomagnets of net spin S = 10 with an Isinglike anisotropy. The degenerate M_{s} = ±S states are split by the ligand electric field into a series of doublets. At temperatures smaller than the level separation, the spins flip by resonant tunnelling through a quasiclassical barrier. The signature of a resonant tunnelling effect in Fe_{8} is a peak in the low temperature relaxation rate around H = 0^{26}. It quickly became clear that to understand the resonant tunnelling both dipolar and dynamic nuclear spin contributions to the interactions need to be accounted for. The typical dipolar field in such a system is ≈0.5 K, and the relevant tunnel splitting ΔE of the order 10^{−8} K, meaning that a broad distribution of dipolar field and a static hyperfine contribution would force all the spins off resonance. Prokof’ev and Stamp^{27} proposed that dynamic nuclear fluctuations can drive the system to resonance, and the gradual adjustment of the dipole fields in the sample caused by tunnelling, brings other clusters into resonance and allows a continuous relaxation. Hence, the observation of relaxation in singlemolecule magnets is fundamentally dependent on the hyperfine coupling with the fields of nuclear spins^{28}.
The Prokof’ev and Stamp model^{27} certainly does not apply in detail to spin ice at low temperatures. First, in singlemolecule magnets the spin of any particular complex in the system is available to be brought to resonance, whereas in spin ice, only those spins that are instantaneously associated with a diffusing monopole are available to tunnel (and this presumes that more extended excitations can be neglected). The remaining spins—the vast majority—are, in contrast, static and instantaneously ordered by the ice rules. The rate of flipping of these quasiordered spins, which corresponds to monopole pair creation, is negligible at the temperatures studied and the process is not relevant to our experiments. Thus, even at equilibrium, spin ice has an effective number of flippable spins that depends on temperature (see Supplementary Fig. 1). Away from equilibrium, where our experiments are performed, the number of flippable spins in spin ice further depends on time, with monopole recombination depleting their number. In addition, it seems reasonable to assume that the reduction of the density of monopoles is even more important during the relaxation process; as monopoles move through the matrix magnetising the sample they will annihilate when they encounter a monopole of opposite charge, or become trapped on a defect or on the sample surface. This feature of spin ice is a second important difference with single molecule magnets, as modelled in ref. ^{27}.
A third difference relates to the distribution of internal fields in the system. In spin ice only, the actual field associated with a flippable spin, both before and after a flip, is a monopolar field. Flipping a spin transfers a monopole from site to site (Fig. 1a), dragging the monopolar field with it: a field that is much stronger and of longer range than any conventional dipole field. However, the change in field on a spin flip is dipolar, as in single molecule magnets.
In short, the flippable spins in spin ice are really an aspect of the emergent monopole excitation rather than a perturbed version of an isolated (composite) spin as assumed for the single molecule magnets in ref. ^{27}. Yet despite this difference, it seems reasonable to suggest that the basic idea of ref. ^{27} does apply to spin ice. The longitudinal monopolar fields will take flippable spins off resonance (Fig. 1c–e), while the transverse ones will tend to broaden the resonance well beyond the tunnel splitting calculated for an isolated spin, i.e., ΔE = 10^{−5} K^{14}. An applied field can also take flippable spins on or off resonance or broaden the resonance, depending on its direction. Nevertheless, in zero applied field, at very low temperatures we would expect all flippable spins associated with isolated monopoles to be off resonance and hence unable to relax, unless they are brought back to resonance by a combination of the monopole fields and the fluctuating nuclear spins: nuclear assisted flipping of spins will then bring further spins to resonance via the change in dipolar fields, as in the Prokof’evStamp picture^{27}. Our experimental results for the wait time dependence of various properties clearly support this proposition: in zero field (during t_{w}) the sample with no nuclear spin is scarcely able to relax its monopole density, while the larger the nuclear spin, the quicker the relaxation. For flippable spins associated with closely spaced monopole–antimonopole pairs the situation is slightly different. Although they are strongly offresonance (Fig. 1b), the decreasing transition matrix elements will be compensated by the increasing Boltzmann factors required for detailed balance. Also, for the final recombination, a favourable change in exchange energy will reduce the field required to bring spins to resonance (see caption, Fig. 1).
We note in passing that the differences between single molecule magnets and spin ice are also evident in our data. Specifically, a t^{1/2} initial relaxation of the magnetisation is a property of singlemolecule magnets, with the t^{1/2} form arising from the dipole interactions^{27,29}. Given the very unusual field distribution in spin ice, and the complicating factor of monopole recombination, as described above, it is hardly likely that this functional form will apply. We test for a t^{1/2} decay in the Supplementary Fig. 5 and confirm that it can only be fitted over a narrow time range: to calculate the true time dependence in spin ice poses a theoretical problem.
Our main result has implications for both the theory of spin ice and the theory of nuclear spin assisted quantum tunnelling. First, in previous work^{11} we have shown how the lowtemperature quenched monopole populations of Dy_{2}Ti_{2}O_{7} obey the nonlinear and nonequlibrium response of monopole theory^{30} that was developed assuming a single hop rate. In view of our findings, the theory should apply most accurately to the Dy_{2}Ti_{2}O_{7} sample with no nuclear spins and least accurately to Ho_{2}Ti_{2}O_{7} where the hyperfine splitting energies are of a similar order to the Coulomb energies. In other measurements, presented in Supplementary Figs. 7 and 8, we confirm that this is the case; hence a generalisation of the theory of ref. ^{30} to include the effect of nuclear spins seems an attainable goal. We also note that Ho_{2}Ti_{2}O_{7} offers the unusual situation that, at low temperatures (<0.35 K) and sufficient wait times, the nuclear spins are icerule ordering antiparallel to their electronic counterparts; hence spin ice offers a rare chance to investigate the effect of correlation on nuclear spin assisted quantum tunnelling in a controlled environment. Perhaps this will shed light on some of the unusual properties particular to Ho_{2}Ti_{2}O_{7}, as noted above.
Spin ice thus exemplifies a remarkable extension of the concept of nuclear spin assisted quantum tunnelling^{27} to the motion of fractionalised topological excitations^{6}. This is made possible by the fact that the emergent excitations of the system—the monopoles—are objects localised in direct space that move through flipping spins. As well as illustrating this generic point, our result may also have practical consequences. We have established how coupling with nuclear spins controls the magnetic monopole current and the spectacular magnetothermal avalanches: hence any experimental handle on the nuclear spins of the system would also be a rare experimental handle on the monopole current. Any future application of magnetic monopoles in spin ice will surely rely on the existence of such experimental handles.
Methods
Samples
Single crystals were grown by the floating zone method for all samples, the natural ^{nat}Dy_{2}Ti_{2}O_{7} and Ho_{2}Ti_{2}O_{7} samples (DTO, HTO) were prepared at the Institute of Solid State Physics, University of Tokyo, Japan, and ^{162}Dy_{2}Ti_{2}O_{7}, ^{163}Dy_{2}Ti_{2}O_{7} at Warwick University and Oxford University, respectively.
Measurements
Measurements were made using a lowtemperature SQUID magnetometer developed at the Institut Néel in Grenoble. The magnetometer is equipped with a miniature dilution refrigerator with a base temperature of 65 mK. The fast dynamics after a field change were measured in a relative mode, the slower measurements were made by the extraction method, and the initial relative measurements were adjusted to the absolute value extraction points. The field could be rapidly changed at a rate up to 2.2 T s^{−1}.
For all the data shown here the field was applied along the [111] crystallographic direction. Measurements were also performed perpendicular to the [111] direction, as well as along the [001] and [011] directions and on a polycrystalline sample, examples of which are discussed in Supplementary Note 3. In total ten different samples were studied. The direction of the applied field as well as differences in the sample shapes and thermal contact with the sample holder can effect some of the details of the measurements. However, this does not change the main conclusion of the paper: the demonstration of the importance of nuclear assisted quantum tunnelling to the relaxation.
The measurements of temperature vs. time shown in Fig. 2, a barechip Cernox 1010BC resistance thermometer from LakeShore Cryogenics was wrapped in Cu foil and glued on top of the sample as shown in the inset of Fig. 2b.
Cooling Ho_{2}Ti_{2}O_{7} was difficult and warming was also tricky using the AQP, depending on the initial temperatures and wait times. Therefore, to ensure the sample was heated above 900 mK, two AQP were used, separated by 300 s, which explains why the starting temperature for Ho_{2}Ti_{2}O_{7} was higher in Fig. 2 (see Supplementary Note 2 and Supplementary Fig. 3 for further discussions).
A schematic of the AQP used for the preparation of the samples is shown in Fig. 3d. First a field of −0.3 T was applied and the sample was allowed to cool to base temperature for 20 min. The field was then reversed at 2.2 T s^{−1} to +0.3 T for 4 s then reduced to zero. After a wait period ranging from 10 to 50,000 s, a field of 0.08 T was applied and the relaxation of the magnetisation was recorded. The field B = 0.08 T was chosen because it is large enough to get sizeable relaxation, but small compared to the avalanche fields shown in Fig. 4. In this way, when applying the magnetic fields, the relaxation is well behaved and the sample does not heat.
The AQP used for the data of Fig. 4 was similar to the above, except the avalanche field was ±0.4 T. After the wait period the field was ramped at 0.02 T s^{−1}, while the magnetisation and temperature of the sample were continuously recorded. For the slow CC protocol measurements shown in Fig. 3, the samples were first heated to 900 mK for 10 s, then cooled at a rate of approximately 0.01 K s^{−1}, followed by a waiting period of 1000 s.
Data availability
Information on the data underpinning the results presented here, including how to access them, can be found in the Cardiff University data catalogue at https://doi.org/10.17035/d.2019.0069144874. The datasets obtained and/or analysed in this study are also available from the corresponding author on reasonable request.
References
 1.
Harris, M. J., Bramwell, S. T., McMorrow, D. F., Zeiske, T. & Godfrey, K. W. Geometrical frustration in the ferromagnetic pyrochlore Ho_{2}Ti_{2}O_{7}. Phys. Rev. Lett. 79, 2554–2557 (1997).
 2.
Bramwell, S. T. & Harris, M. J. Frustration in Isingtype spin models on the pyrochlore lattice. J. Phys. Condens. Matter 10, L215–L220 (1998).
 3.
Ramirez, A. P., Hayashi, A., Cava, R. J., Siddharthan, R. B. & Shastry, S. Zeropoint entropy in spin ice. Nature 399, 333–335 (1999).
 4.
Bramwell, S. T. & Gingras, M. J. P. Spin ice state in frustrated magnetic pyrochlore materials. Science 294, 1495–1501 (2001).
 5.
Luttinger, J. M. & Tisza, L. Theory of dipole interactions in crystals. Phys. Rev. 70, 954–964 (1946).
 6.
Castelnovo, C., Moessner, R. & Sondhi, S. L. Magnetic monopoles in spin ice. Nature 451, 42–45 (2008).
 7.
den Hertog, B. C. & Gingras, M. J. P. Dipolar interactions and origin of spin ice in Ising pyrochlore magnets. Phys. Rev. Lett. 84, 3430–3433 (2000).
 8.
Isakov, S. V., Moessner, R. & Sondhi, S. L. Why spin ice obeys the ice rules. Phys. Rev. Lett. 95, 217201 (2005).
 9.
Ryzhkin, I. A. Magnetic relaxation in rareearth pyrochlores. J. Exp. Theor. Phys. 101, 481–486 (2005).
 10.
Kaiser, V. et al. Emergent electrochemistry in spin ice: Debye–Hückel theory and beyond. Phys. Rev. B 98, 144413 (2018).
 11.
Paulsen, C. et al. Experimental signature of the attractive Coulomb force between positive and negative magnetic monopoles in spin ice. Nat. Phys. 12, 661–666 (2016).
 12.
Jaubert, L. D. C. & Holdsworth, P. C. W. Signature of magnetic monopole and Dirac string dynamics in spin ice. Nat. Phys. 5, 258–261 (2009).
 13.
Bovo, L., Bloxsom, J. A., Prabhakaran, D., Aeppli, G. & Bramwell, S. T. Brownian motion and quantum dynamics of magnetic monopoles in spin ice. Nat. Comms. 4, 1535 (2013).
 14.
Tomasello, B., Castelnovo, C., Messier, R. & Quintanilla, J. Singleion anisotropy and magnetic field response in the spinice materials Ho_{2}Ti_{2}O_{7} and Dy_{2}Ti_{2}O_{7}. Phys. Rev. B 92, 155120 (2015).
 15.
Vedmedenko, E. Y. Dynamics of bound monopoles in artificial spin ice: how to store energy in Dirac strings. Phys. Rev. Lett. 116, 077202 (2016).
 16.
Melko, R. G., den Hertog, B. C. & Gingras, M. J. P. Long range order at low temperatures in dipolar spin ice. Phys. Rev. Lett. 87, 067203 (2001).
 17.
Ehlers, G. et al. Evidence for two distinct spin relaxation mechanisms in ‘hot’ spin ice Ho_{2}Ti_{2}O_{7}. J. Phys. Condens. Matter 16, S635–S642 (2004).
 18.
Snyder, J. et al. Lowtemperature spin freezing in the Dy_{2}Ti_{2}O_{7} spin ice. Phys. Rev. B 69, 064414 (2004).
 19.
Castelnovo, C., Moessner, R. & Sondhi, S. L. Thermal quenches in spin ice. Phys. Rev. Lett. 104, 107201 (2010).
 20.
Paulsen, C. et al. Farfromequilibrium monopole dynamics in spin ice. Nat. Phys. 10, 135–139 (2014).
 21.
Planck Collaboration. Planck early results. II. The thermal performance of Planck. Astron. Astrophys. 536, A2 (2011).
 22.
Slobinsky, D. et al. Unconventional magnetization processes and thermal runaway in spinice Dy_{2}Ti_{2}O_{7}. Phys. Rev. Lett. 105, 267205 (2010).
 23.
Jackson, M. J. et al. Dynamic behavior of magnetic avalanches in the spinice compound Dy_{2}Ti_{2}O_{7}. Phys. Rev. B 90, 064427 (2014).
 24.
Krey, C. et al. First order metamagnetic transition in Ho_{2}Ti_{2}O_{7} observed by vibrating coil magnetometry at Milli–Kelvin temperatures. Phys. Rev. Lett. 108, 257204 (2012).
 25.
Gatteschi, D. & Sessoli, R. Quantum tunneling of magnetization and related phenomena in molecular materials. Angew. Chem. 42, 268–297 (2003).
 26.
Sangregorio, C., Ohm, T., Paulsen, C., Sessoli, R. & Gatteschi, D. Quantum tunneling of the magnetization in an Iron cluster nanomagnet. Phys. Rev. Lett. 78, 4645–4648 (1997).
 27.
Prokof’ev, N. V. & Stamp, P. C. E. Lowtemperature quantum relaxation in a system of magnetic nano molecules. Phys. Rev. Lett. 80, 5794–5797 (1998).
 28.
Wernsdorfer, W. et al. Effects of nuclear spins on the quantum relaxation of the magnetization for the molecular nanomagnet Fe_{8}. Phys. Rev. Lett. 84, 2965–2968 (2000).
 29.
Ohm, T., Sangregorio, C. & Paulsen, C. Nonexponential relaxation in a resonant quantum tunneling system of magnetic molecules. J. Low Temp. Phys. 113, 1141–1146 (1998). https://doi.org/10.1023/A:1022545510114.
 30.
Kaiser, V., Bramwell, S. T., Holdsworth, P. C. W. & Moessner, R. ac Wien effect in spin ice, manifest in nonlinear, nonequilibrium susceptibility. Phys. Rev. Lett. 115, 037201 (2015).
Acknowledgements
S.R.G. thanks Cardiff University for ‘seedcorn’ funding, and acknowledges the EPSRC for EP/L019760/1 and EP/S016465/1. S.T.B. thanks Patrik Henelius for communicating his independent ideas on nuclear assisted quantum tunnelling in spin ice, and acknowledges the EPSRC for EP/S016554/1. E.L. and C.P. acknowledge financial support from ANR, France, Grant no. ANR15CE300004. G.B. wishes to thank financial support from EPSRC, UK, through grant EP/M028771/1.
Author information
Affiliations
Contributions
The experiments were designed and performed by C.P. with inputs and discussions from E.L. and S.R.G. The data were analysed by C.P., E.L., S.R.G. and S.T.B. Contributed materials were fabricated by K.M., D.P. and G.B. The paper was written by C.P., E.L., S.R.G. and S.T.B.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Journal peer review information: Nature Communications thanks the anonymous reviewers for their contribution to the peer review of this work. Peer reviewer reports are available.
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Paulsen, C., Giblin, S.R., Lhotel, E. et al. Nuclear spin assisted quantum tunnelling of magnetic monopoles in spin ice. Nat Commun 10, 1509 (2019). https://doi.org/10.1038/s41467019093236
Received:
Accepted:
Published:
Further reading

Screening and the pinch point paradox in spin ice
Physical Review Research (2020)

The history of spin ice
Journal of Physics: Condensed Matter (2020)

Extremely slow nonequilibrium monopole dynamics in classical spin ice
Physical Review B (2020)

Quantum Versus Classical Spin Fragmentation in Dipolar Kagome Ice Ho3Mg2Sb3O14
Physical Review X (2020)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.